Download (direct link):
strength of donor and acceptor groups significantly increase the />
value. The [1 value varied slightly as a function of aryl group
composition lor a series of compounds with phenylamine donors and
nitrophenyl or nitrophenylethynyl-acceptor groups.
LeC'oers et al.!' synthesized push-pull arylethynyl porphyrins and
measured their fi values by hyper-Rayleigh scattering (I IRS) in
chloroform solutions. The donor-acceptor compound D-Zn( DPP)-A produced
approximately frequency independent ji values: 5142 x 10 esu at 830 nm
and 4933 * 10 esu al 1064nm. The copper
analogue (D-Cu( 1 )PP))-A) exhibited frequency-dependent values of 4374 x
10 " esu at 830 nm and 1501 x 10 10 esu al 1064 nm. Significant shifts in
molecular dipole moment were observed for the push-pull arylethynyl
porphyrins by electroabsoiption or Stark effect spectro-scopv.w The //
value of the zinc porphyrin dimer D-Zn(L)PP)-Zn(DPP)-A calculated at 1064
nm was 742 x It) '(icni'/esu (Figure 28). The calculated fi/f value at
I907 nm was 3299 a 10 lscm7esu. The /)' value of I) Z.n(DPP)-Zn(DPPl-A is
1.6 times larger than that of l)-Zinl)PP)-A. The larger /> value is
associated with two ZmDPPl units linked together bv an ethynyl bridge
connecting the chromophores at their 5 and 5'-positions.
The lirsi nickel push-pull 5.15-diphenylporphyrin deriv atives were
recently synthesized by Yeung.|S Using an amino arylethynyl group as Ihe
donor substituent and a lormyl or a dicvaiioethynyl group as the acceptor
Chou et al.
Table 5. INDO/SCI-SOS Calculated /i Values at 1064nm for Porphyrin-
Bridged Donor-Acceptor Molecules
D= - <Q^N(CH,)2 ; ë=- = ^ ^N0,
No. Porphyrins R1 R2 R3 R4 M p (10 30 esu)
1 Zn(DPP) Ph H Ph H Zn ---
2 D-Zn(DPP) Ph D Ph H Zn 106.7
3 Zn(DPP)-A Ph H Ph A Zn 147.5
4 D-Zn(DPP)-A Ph D Ph A Zn 477.3
5 d-Hi(DPP)-A Ph d PIi a H, 50.9
6 di-Hi(P)-a5 d d a a H, 95.3
7 ñÖ-Í-.(Ð)-à d d d a Ht 53.6
8 d-H2(P)-a( d a a a Hb 65.2
Source: Priyadarshy. S.; Thericn. M. J.; Beratan, D. N. J. Am. Chem. Soc.
1996. 118. 1504.
Figure 28. Structure of LeCoer's zinc porphyrin dimer.
the porphyrin, the nickel-containing species exhibited significant first
hyperpolarizability. Using EFISH at 1907 öø, the first
hyperpolarizabilities were determined as 124 x 10 ~ 30 esu and 66 x 10 30
esu for the formyl and dicyanoethynyl species, respectively. The larger
ft value for dicyanoethynyl compound is attributed to its higher relative
electronic acceptor strength.
Albert et al.46 calculated [j values of push-pull porphyrins using
semi-empirical INDO/S Hamiltonian and singles-only Cl (Table 6). The
calculated optimized j8 values and chemical structures are therein. The
ft value increased as the benzene ring was replaced by an electron-
deficient moiety such as diazene or tetra-azine or by an electron-rich
ring such as thiophene or pyrrole. The j8vcl. and ftp increased by a
factor of two by replacing the benzene rings at the donor end by
electron-donating pyrrole rings. A series of porphyrins with reduced
dihedral twist of the phenyl rings were synthesized and present very
large fl values. Small dihedral angles were observed for the alkyne
bridged (7 °) and for the azo-bridged species (0.5).
A multifunctional polyimide consisting of a free-base porphyrin and a
NLO chromophore side chain was synthesized by Peng and associates (Figure
29).47 This photorefractive molecular system was modeled on the charge-
transfer properties observed in porphyrin electron acceptors of
photosynthetic processes. The polyimide exhibited a Tg of 250 °C.
Absorption peaks at 510, 540 and 630nm from the porphyrin rings and at
458 nm from the NLO-chromophore were observed. This multifunctional
polyimide system is photoconductive as well as SHG active. The
photoconductivity was determined to be 1.1 x 10 ~ 12 S/cm under an
external field of 1500kV/cm at 690 nm. The polymer film showed a NLO
coefficient d33 of 110pm/Vat 1.064 öò after corona poling. Interestingly,
the NLO coefficient d33 showed no decay at 90 and 150 °C, and the d33 of
80% was retained even at 170 °C after 120 hours. This porphyrin-
containing polyimide displayed a higher NLO coefficient as well as
stability of second harmonic generation at high temperature. Additional
photorefractive effects were observed in the two-beam coupling
41 / Porphyrin Materials Chemistry
An optical gain coefficient of 22.2 cm - under zero-field condition was
Another new photorefractive polyimide (Figure 30) with a main-chain
zinc porphyrin (m = 0.005) and a NLO-chromophore side chain (n = 0.995)
was reported by Peng el a/.4X This porphyrin-containing fluorinated
polyimide displayed a T" of 228 °C and maintained thermal stability to
350 °C. The photoconductivity was found to be electric-field dependent.